#------------------------------------------------------------------------------
#$Date: 2014-08-15 21:12:14 +0300 (Fri, 15 Aug 2014) $
#$Revision: 22 $
#$URL: svn://svn.code.sf.net/p/propcif/code/trunk/cif/1/1000001.mpod $
#------------------------------------------------------------------------------
#
# This file is available in the Material Properties Open Database (MPOD),
# http://www.mpod.net/
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_1000001
_cod_database_code ?
_structure_refined 'no'
_mpod_phase_name 'Al72Ni16Co8'
_chemical_formula_sum 'Al72 Ni16 Co8'
_mpod_symmetry_point_group_name_H-M 10mm
_cell_length_a ?
loop_
_publ_author_name
'Tarumi R.'
'Ledbetter H.'
'Shiomi S.' 
'Ogi H.'
'Hirao M.'
'Tsai A.P.'
_publ_section_title
;
 Elastic constants and anisotropic internal frictions of decagonal Al72Ni18Co8 single quasicrystal at low temperature
;
_journal_name_full               'Journal of Applied Physics'
_journal_volume                  108
_journal_issue                   1
_journal_article_reference       013514
_journal_pages_number            5
_journal_year                    2010
_prop_measurement_method 'EMAR'
_prop_elastic_stiffness_cij 'cij'
_prop_internal_friction_Qij-1 'Qij-1'
loop_
_prop_data_label
_prop_data_tensorial_index
_prop_data_value
_prop_conditions_temperature
cij 11 229.0 290
cij 12 ? 290
cij 13 59.6 290
cij 22 229.0 290
cij 23 59.6 290
cij 33 221.9 290
cij 44 69.3 290
cij 55 69.3 290
cij 66 85.8 290
Qij-1 11 2.7 290
Qij-1 12 ? 290
Qij-1 13 ? 290
Qij-1 22 2.7 290
Qij-1 23 ? 290
Qij-1 33 26.5 290
Qij-1 44 3.2 290
Qij-1 55 3.2 290
Qij-1 66 5.4 290
cij 11 235.9 5
cij 12 ? 5
cij 13 61.3 5
cij 22 235.9 5
cij 23 59.6 5
cij 33 234.5 5
cij 44 72.2 5
cij 55 72.2 5
cij 66 89.6 5
Qij-1 11 0.4 5
Qij-1 12 ? 5
Qij-1 13 ? 5
Qij-1 22 0.4 5
Qij-1 23 ? 5
Qij-1 33 9.6 5
Qij-1 44 2.0 5
Qij-1 55 2.0 5
Qij-1 66 2.3 5